Shielded metal arc welding (SMAW), • Also known as Manual Metal Arc (MMA) welding • Informally as stick welding • is a manual arc welding process that uses a consumable electrode coated in flux to lay the weld. • An electric current, in the form of either alternating current or direct current from a welding power supply, is used to form an electric arc between the electrode and the metals to be joined.
As the weld is laid, the flux coating of the electrode disintegrates, giving off vapors that serve as a shielding gas and providing a layer of slag, both of which protect the weld area from atmospheric contamination. • Because of the versatility of the process and the simplicity of its equipment and operation, shielded metal arc welding is one of the world's most popular welding processes.
It dominates other welding processes in the maintenance and repair industry, used extensively in the construction of steel structures and in industrial fabrication. • The process is used primarily to weld iron and steels (including stainless steel) but aluminum, nickel and copperalloys can also be welded with this method. • Flux-Cored Arc Welding (FCAW) , a modification to SMAW is growing in popularity
SAFETY PRECAUTIONS • Uses an open electric arc, so risk of burns – to be prevented by protective clothing in the form of heavy leathergloves and long sleeve jackets. • The brightness of the weld area can lead arc eye, in which ultraviolet light causes the inflammation of the cornea and can burn the retinas of the eyes. • Welding helmets with dark face plates to be worn to prevent this exposure
New helmet models have been produced that feature a face plate that self-darkens upon exposure to high amounts of UV light • To protect bystanders, especially in industrial environments, transparent welding curtains often surround the welding area. • These are made of a polyvinyl chloride plastic film, shield nearby workers from exposure to the UV light from the electric arc, but should not be used to replace the filter glass used in helmets.
Arc eye, also known as arc flash or welder's flash or corneal flash burns, is a painful condition sometimes experienced by welders who have failed to use adequate eye protection. It can also occur due to light from sunbeds, light reflected from snow (known as snow blindness), water or sand. The intense ultraviolet light emitted by the arc causes a superficial and painful keratitis. Symptoms tend to occur a number of hours after exposure and typically resolve spontaneously within 36 hours. It has been described as having sand poured into the eyes. ARC EYE
SignsIntense lacrimationBlepharospasmPhotophobiaFluorescein dye staining will reveal corneal ulcers under blue light Management • Instill topical anaesthesia • Inspect the cornea for any foreign body • Patch the worse of the two eyes and prescribe analgesia • Topical antibiotics in the form of eye drops or eye ointment or both should be prescribed for prophylaxis against infection
Submerged Arc Welding (SAW) • Is a common arc welding process. • A continuously fed consumable solid or tubular (metal cored) electrode used. • The molten weld and the arc zone are protected from atmospheric contamination by being “submerged” under a blanket of granular fusible flux. • When molten, the flux becomes conductive, and provides a current path between the electrode and the work
Normally operated in the automatic or mechanized mode. • Semi-automatic (hand-held) SAW guns with pressurized or gravity flux feed delivery are available. • The process is normally limited to the 1F, 1G, or the 2F positions (although 2G position welds have been done with a special arrangement to support the flux). Deposition rates approaching 45 kg/h have been reported — this compares to ~5 kg/h (max) for shielded metal arc welding. • Currents ranging from 200 to 1500 A are commonly used; currents of up to 5000 A have been used (multiple arcs).
Single or multiple (2 to 5) electrode wire variations of the process exist • SAW strip-cladding utilizes a flat strip electrode (e.g. 60 mm wide x 0.5 mm thick). • DC or AC power can be utilized, and combinations of DC and AC are common on multiple electrode systems. • Constant Voltage welding power supplies are most commonly used, however Constant Current systems in combination with a voltage sensing wire-feeder are available.
Material applications • Carbon steels (structural and vessel construction); • Low alloy steels; • Stainless Steels; • Nickel-based alloys; • Surfacing applications (wearfacing, build-up, and corrosion resistant overlay of steels).
Advantages of SAW • High deposition rates (over45 kg/h) have been reported; • High operating factors in mechanized applications; • Deep weld penetration; • Sound welds are readily made (with good process design and control); • High speed welding of thin sheet steels at over 2.5 m/min is possible; • Minimal welding fume or arc light is emitted.
Limitations of SAW • Limited to ferrous (steel or stainless steels) and some nickel based alloys; • Normally limited to the 1F, 1G, and 2F positions; • Normally limited to long straight seams or rotated pipes or vessels; • Requires relatively troublesome flux handling systems; • Flux and slag residue can present a health & safety issue; • Requires inter-pass and post weld slag removal.
Key SAW process variables • Wire Feed Speed (main factor in welding current control); • Arc Voltage; • Travel Speed; • Electrical Stick-Out (ESO) or Contact Tip to Work (CTTW); • Polarity and Current Type (AC or DC). Other factors • Flux depth/width; • Flux and electrode classification and type; • Electrode wire diameter; • Multiple electrode configurations.
GTAW • Fusion Welding Process • Arc Between Non-Consumable Tungsten Rod And Work • Arc & Weld Pool Shielded By Argon/Gas • Filler Wire Separately Added To Weld Pool • Welding Torch & Tungsten Rod Cooled by Flow OF Argon / Cooling Water
GTAW Equipment & Accessories • Power Source – Inverter, Thyrister, Rectifier, Generator • High Frequency Unit • Water Cooling System • Welding Torch-(Ceramic Cup, Tungsten Rod, Collet, Gas-lens) • Pedal Switch • Argon Gas Cylinder • Pressure Gauge, Regulator, Flow Meter • Earthing Cable With Clamp
Equipment & Accessories Pressure Regulator Flow Meter Tungsten Rod Argon Gas In Solenoid Valve Cooling Water In Argon Cylinder Gas Lens HF Unit & Water Cooling System Welding Cable & Cooling Water In Tube Ceramic Cup Cooling Water Out Argon Shielding Arc High Frequency Connection + Work Pedal Switch Power Source – +
Equipment GTAW torch with various electrodes, cups, collets and gas diffusers GTAW torch, disassembled
Gas tungsten arc welding (GTAW), commonly known as Tungsten Inert Gas (TIG) welding • Is an arc welding process that uses a nonconsumable tungstenelectrode to produce the weld. • The weld area is protected from atmospheric contamination by a shielding gas (usually an inert gas such as argon), and a filler metal is normally used, though some welds, known as autogenous welds, do not require it. • A constant current welding power supply produces energy which is conducted across the arc through a column of highly ionized gas and metal vapors known as a plasma.
Most commonly used to weld thin sections of stainless steel and light metals such as aluminum, magnesium, and copper alloys. • The process grants the operator greater control over the weld than competing procedures such as shielded metal arc welding and gas metal arc welding, allowing for stronger, higher quality welds. • GTAW is comparatively more complex and difficult to master, and furthermore, it is significantly slower than most other welding techniques. • A related process, plasma arc welding, uses a slightly different welding torch to create a more focused welding arc and as a result is often automated.
Applications • Aerospace industry is one of the primary users of gas tungsten arc welding, the process is used in a number of other areas. • Many industries use GTAW for welding thin workpieces, especially nonferrous metals. • It is used extensively in the manufacture of space vehicles, and is also frequently employed to weld small-diameter, thin-wall tubing. • Is often used to make root or first pass welds for piping of various sizes. • In maintenance and repair work, the process is commonly used to repair tools and dies, especially components made of aluminum and magnesium. • Because the welds it produces are highly resistant to corrosion and cracking over long time periods, GTAW is the welding procedure of choice for critical welding operations like sealing spent nuclear fuel canisters before burial.
GTAW ranks the highest in terms of the quality of weld produced. Operation must be with free from oil, moisture, dirt and other impurities, as these cause weld porosity and consequently a decrease in weld strength and quality. To remove oil & grease, alcohol or similar commercial solvents used, while a stainless steel wire brush or chemical process remove oxides from the surfaces of metals like aluminum. Rust on steels removed by first grit blasting the surface and then using a wire brush to remove imbedded grit. These steps important when DCEN used, because this provides no cleaning during the welding process, unlike DCEPor AC. Quality To maintain a clean weld pool during welding, the shielding gas flow should be sufficient and consistent so that the gas covers the weld and blocks impurities in the atmosphere. GTA welding in windy or drafty environments increases the amount of shielding gas necessary to protect the weld, increasing the cost and making the process unpopular outdoors.
Because of GTAW's relative difficulty and the importance of proper technique, skilled operators are employed for important applications. • Low heat input, caused by low welding current or high welding speed, can limit penetration and cause the weld bead to lift away from the surface being welded. • If there is too much heat input, the weld bead grows in width while the likelihood of excessive penetration and spatter increase. • If the welder holds the welding torch too far from the workpiece, shielding gas is wasted and the appearance of the weld worsens.
If the amount of current used exceeds the capability of the electrode, tungsten inclusions in the weld may result. Known as tungsten spitting, it can be identified with radiography and prevented by changing the type of electrode or increasing the electrode diameter. • If the electrode is not well protected by the gas shield or the operator accidentally allows it to contact the molten metal, it can become dirty or contaminated. This often causes the welding arc to become unstable, requiring that electrode be ground with a diamond abrasive to remove the impurity.
GTAW welding torches designed for either automatic or manual operation and are equipped with cooling systems using air or water. The automatic and manual torches are similar in construction, but the manual torch has a handle while the automatic torch normally comes with a mounting rack. • The angle between the centerline of the handle and the centerline of the tungsten electrode, known as the head angle, can be varied on some manual torches according to the preference of the operator. • Air cooling systems are most often used for low-current operations (up to about 200 A), while water cooling is required for high-current welding (up to about 600 A). • The torches are connected with cables to the power supply and with hoses to the shielding gas source and where used, the water supply.
The internal metal parts of a torch are made of hard alloys of copper or brass in order to transmit current and heat effectively. • The tungsten electrode must be held firmly in the center of the torch with an appropriately sized collet, and ports around the electrode provide a constant flow of shielding gas. • The body of the torch is made of heat-resistant, insulating plastics covering the metal components, providing insulation from heat and electricity to protect the welder.
GTAW TORCH Torch Handle Cap with collet For Holding Tungsten Cooling Water Outlet Argon Gas Inlet Cooling Water Inlet Tube with cable Ceramic Cup Argon Shielding Gas Tungsten Rod Base Metal Earthing Cable Arc
The size of the welding torch nozzle depends on the size of the desired welding arc, and the inside diameter of the nozzle is normally at least three times the diameter of the electrode. • The nozzle must be heat resistant and thus is normally made of alumina or a ceramic material, but fused quartz, a glass-like substance, offers greater visibility. • Devices can be inserted into the nozzle for special applications, such as gas lenses or valves to control shielding gas flow and switches to control welding current.
Power supply • GTAW uses a constant current power source, meaning that the current (and thus the heat) remains relatively constant, even if the arc distance and voltage change. • This is important because most applications of GTAW are manual or semiautomatic, requiring that an operator hold the torch. • Maintaining a suitably steady arc distance is difficult if a constant voltage power source is used instead, since it can cause dramatic heat variations and make welding more difficult.
The preferred polarity of the GTAW system depends largely on the type of metal being welded. • DCEN is often employed when welding steels, nickel, titanium, and other metals. It can also be used in automatic GTA welding of aluminum or magnesium when helium is used as a shielding gas. The negatively charged electrode generates heat by emitting electrons which travel across the arc, causing thermal ionization of the shielding gas and increasing the temperature of the base material. The ionized shielding gas flows toward the electrode, not the base material, and this can allow oxides to build on the surface of the weld. • DCEP is less common, and is used primarily for shallow welds since less heat is generated in the base material. Instead of flowing from the electrode to the base material, as in DCEN, electrons go the other direction, causing the electrode to reach very high temperatures. To help it maintain its shape and prevent softening, a larger electrode is often used. As the electrons flow toward the electrode, ionized shielding gas flows back toward the base material, cleaning the weld by removing oxides and other impurities and thereby improving its quality and appearance.
AC commonly used when welding aluminum and magnesium manually or semi-automatically, combines the two direct currents by making the electrode and base material alternate between positive and negative charge. This causes the electron flow to switch directions constantly, preventing the tungsten electrode from overheating while maintaining the heat in the base material. This makes the ionized shielding gas constantly switch its direction of flow, causing impurities to be removed during a portion of the cycle. • Some power supplies enable operators to use an unbalanced alternating current wave by modifying the exact percentage of time that the current spends in each state of polarity, giving them more control over the amount of heat and cleaning action supplied by the power source. • In addition, operators must be wary of rectification, in which the arc fails to reignite as it passes from straight polarity (negative electrode) to reverse polarity (positive electrode). • To remedy the problem, a square wave power supply can be used, as can high frequency voltage to encourage ignition.
Tungsten Rod Tungsten Rod • Non Consumable Electrode. • Maintains Stable Arc • Tip to be Ground to a cone Shape of 60º to 30º angle • Thoriated Tungsten for General Application, Zerconiated Tungsten for Aluminium Welding • Sizes :- 2, 2.4& 3 mm Ø Ground to 50º ankle
The electrode used in GTAW is made of tungsten or a tungsten alloy, because tungsten has the highest melting temperature among metals, at 3422 °C. • The electrode is not consumed during welding, though some erosion (called burn-off) can occur. • Electrodes can have either a clean finish or a ground finish—clean finish electrodes have been chemically cleaned, while ground finish electrodes have been ground to a uniform size and have a polished surface, making them optimal for heat conduction. • The diameter of the electrode can vary between 0.5 mm and 6.4 mm, and their length can range from 75 to 610 mm .
A number of tungsten alloys have been standardized by the International Organization for Standardization and the American Welding Society in ISO 6848 and AWS A5.12, respectively, for use in GTAW electrodes- refer table • Pure tungsten electrodes (classified as WP or EWP) are general purpose and low cost electrodes. Cerium oxide (or ceria) as an alloying element improves arc stability and ease of starting while decreasing burn-off. Using an alloy of lanthanum oxide (or lanthana) has a similar effect. Thorium oxide (or thoria) alloy electrodes were designed for DC applications and can withstand somewhat higher temperatures while providing many of the benefits of other alloys. • However, it is somewhat radioactive, and as a replacement, electrodes with larger concentrations of lanthanum oxide can be used. Electrodes containing zirconium oxide (or zirconia) increase the current capacity while improving arc stability and starting and increasing electrode life. • Electrode manufacturers may create alternative tungsten alloys with specified metal additions, and these are designated with the classification EWG under the AWS system. • Filler metals are also used in nearly all applications of GTAW, the major exception being the welding of thin materials. Filler metals are available with different diameters and are made of a variety of materials. In most cases, the filler metal in the form of a rod is added to the weld pool manually, but some applications call for an automatically fed filler metal, which is fed from rolls.
shielding gases • Necessary in GTAW to protect the welding area from atmospheric gases such as nitrogen and oxygen, which can cause fusion defects, porosity, and weld metal embrittlement if they come in contact with the electrode, the arc, or the welding metal. The gas also transfers heat from the tungsten electrode to the metal, and it helps start and maintain a stable arc. • The selection of a shielding gas depends on several factors, including the type of material being welded, joint design, and desired final weld appearance. • Argon is the most commonly used shielding gas for GTAW, since it helps prevent defects due to a varying arc length. When used with alternating current, the use of argon results in high weld quality and good appearance. • Another common shielding gas, helium, is most often used to increase the weld penetration in a joint, to increase the welding speed, and to weld conductive metals like copper and aluminum. • A significant disadvantage is the difficulty of striking an arc with helium gas, and the decreased weld quality associated with a varying arc length.
Shielding Gas • Inert Gas - Argon , Helium • Common Shielding Gas – Argon • When Helium Is Used – Called Heli – Arc Welding • When Argon Is Used – Called Argon Arc Welding • Inert Gas Prevents Contamination Of Molten Metal • It Prevents Oxidation Of Tungsten Rod • It Ionizes Air Gap and Stabilizes Arc • It Cools Welding Torch & Tungsten Rod
Shielding Gas • Argon - Purity 99.95% • Impure Argon Results In Porosities • Purity Verified by Fusing BQ CS plate • Leakage of Argon in Torch Results in Porosity. • Check Leakage by Closing the Ceramic Cup With Thump
Argon Gas Cylinder • Light Blue In Colour • Full Cylinder Pressure: 1800 psi ( 130 Kgs / Cm2 ) • Volume Of Argon In Full Cylinder: 7.3 M3 • Commercial Argon (99.99%) Cost: Rs 70/- Per M3 • High Purity Argon (99.999) Cost: Rs 87/- Per M3
Purging Gas Commercial Argon or Nitrogen Applicable to Single Sided full penetration Prevents oxidation of root pass from opposite side of weld Essential for high alloy steels, nonferrous metals and alloys Desirable For All Material Back Purging Filler Wire Welding Torch Purging Gas Out Purging Gas In Root Pass Purging chamber
Argon-helium mixtures are also frequently utilized in GTAW, since they can increase control of the heat input while maintaining the benefits of using argon. Normally, the mixtures are made with primarily helium (often about 75% or higher) and a balance of argon. These mixtures increase the speed and quality of the AC welding of aluminum, and also make it easier to strike an arc. • Argon-hydrogen, is used in the mechanized welding of light gauge stainless steel, but because hydrogen can cause porosity, its uses are limited. • Nitrogen can sometimes be added to argon to help stabilize the austenite in austentitic stainless steels and increase penetration when welding copper. Due to porosity problems in ferritic steels and limited benefits, however, it is not a popular shielding gas additive.
Materials • Most commonly used to weld stainless steel and nonferrous materials, such as aluminum and magnesium, but it can be applied to nearly all metals, with notable exceptions being lead and zinc. • Its applications involving carbon steels are limited not because of process restrictions, but because of the existence of more economical steel welding techniques, such as gas metal arc welding and shielded metal arc welding. • GTAW can be performed in a variety of other-than-flat positions, depending on the skill of the welder and the materials being welded.